#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:56:04 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180523 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/92/7219297.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7219297
loop_
_publ_author_name
'Jiao, Yan-Qing'
'Qin, Chao'
'Zang, Hong-Ying'
'Chen, Wei-Chao'
'Wang, Chun-Gang'
'Zheng, Tian-Tian'
'Shao, Kui-Zhan'
'Su, Zhong-Min'
_publ_section_title
;
 Assembly of organic--inorganic hybrid materials constructed from
 polyoxometalate and metal--1,2,4-triazole units: synthesis, structures,
 magnetic, electrochemical and photocatalytic properties
;
_journal_issue                   10
_journal_name_full               CrystEngComm
_journal_page_first              2176
_journal_paper_doi               10.1039/C4CE02007C
_journal_volume                  17
_journal_year                    2015
_chemical_formula_moiety         'C20 H48 N30 O98 Si2 W24 Zn5'
_chemical_formula_sum            'C20 H48 N30 O98 Si2 W24 Zn5'
_chemical_formula_weight         7072.11
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_block_doi                 10.5517/cc13893s
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;
_cell_angle_alpha                99.833(5)
_cell_angle_beta                 99.520(5)
_cell_angle_gamma                101.798(5)
_cell_formula_units_Z            1
_cell_length_a                   13.0880(5)
_cell_length_b                   13.7640(5)
_cell_length_c                   15.9630(5)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.000
_cell_measurement_theta_min      1.90
_cell_volume                     2713.05(19)
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0587
_diffrn_reflns_av_sigmaI/netI    0.1131
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            14228
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.87
_exptl_absorpt_coefficient_mu    26.551
_exptl_absorpt_correction_T_max  0.004
_exptl_absorpt_correction_T_min  0.002
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.322
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3106
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.20
_refine_diff_density_max         3.366
_refine_diff_density_min         -2.529
_refine_diff_density_rms         0.504
_refine_ls_extinction_coef       0.00016(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     809
_refine_ls_number_reflns         9447
_refine_ls_number_restraints     503
_refine_ls_restrained_S_all      0.983
_refine_ls_R_factor_all          0.1062
_refine_ls_R_factor_gt           0.0574
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0512P)²+31.2380P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1156
_refine_ls_wR_factor_ref         0.1401
_reflns_number_gt                6075
_reflns_number_total             9447
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            c4ce02007c2.cif
_cod_data_source_block           2
_cod_depositor_comments
'Adding full bibliography for 7219296--7219301.cif.'
_cod_original_cell_volume        2713.05(5)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7219297
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
O1 O 0.1111(15) 0.8456(13) 0.6334(11) 0.032(5) Uani 1 1 d .
O2 O 0.2593(13) 0.9750(11) 0.9377(10) 0.019(4) Uani 1 1 d U
O3 O 0.2181(13) 0.8183(12) 0.7906(11) 0.022(4) Uani 1 1 d .
O4 O 0.3324(13) 0.8620(11) 0.6776(10) 0.019(4) Uani 1 1 d .
O5 O 0.4075(12) 0.9285(10) 0.8410(10) 0.015(4) Uani 1 1 d .
O6 O 0.5286(14) 0.8790(12) 0.6440(11) 0.026(4) Uani 1 1 d .
O7 O 0.6084(12) 0.9478(11) 0.8133(10) 0.015(4) Uani 1 1 d U
O6W O -0.2616(14) 0.1340(13) 0.7296(12) 0.037(5) Uani 1 1 d .
H6WC H -0.2382 0.1211 0.7784 0.044 Uiso 1 1 d R
H6WD H -0.2936 0.1814 0.7385 0.044 Uiso 1 1 d R
O8 O 0.0930(12) 0.6591(11) 0.6751(10) 0.018(4) Uani 1 1 d U
O7W O -0.1793(18) 0.2890(15) 0.6354(16) 0.060(7) Uani 1 1 d .
O9 O 0.4193(13) 0.8805(11) 0.9978(10) 0.018(4) Uani 1 1 d U
O8W O 0.1941(15) 0.1561(12) 0.9163(12) 0.032(5) Uani 1 1 d .
H8WC H 0.2203 0.1050 0.9202 0.039 Uiso 1 1 d R
H8WD H 0.1359 0.1465 0.9341 0.039 Uiso 1 1 d R
O10 O 0.2117(13) 0.6998(11) 0.5589(10) 0.021(4) Uani 1 1 d U
O9W O 0.2666(14) 0.0965(14) 0.7520(12) 0.035(5) Uani 1 1 d .
H9WC H 0.2993 0.1311 0.8021 0.042 Uiso 1 1 d R
O11 O 0.6243(16) 0.7560(12) 0.5469(11) 0.030(5) Uani 1 1 d .
O12 O 0.2527(14) 0.5469(12) 0.4454(10) 0.024(4) Uani 1 1 d U
O13 O 0.4138(12) 0.6887(11) 0.5710(10) 0.017(4) Uani 1 1 d U
O14 O 0.6776(13) 0.8004(11) 0.7246(10) 0.021(4) Uani 1 1 d U
O15 O 0.1598(13) 0.5133(11) 0.5842(10) 0.022(4) Uani 1 1 d U
O16 O 0.2908(13) 0.6555(11) 0.6999(10) 0.014(4) Uani 1 1 d .
O17 O 0.5900(13) 0.8366(11) 0.9367(10) 0.020(4) Uani 1 1 d U
O18 O 0.5716(13) 0.8148(12) 1.1081(10) 0.025(4) Uani 1 1 d .
O19 O 0.7888(13) 0.8915(11) 0.8920(11) 0.024(4) Uani 1 1 d .
O20 O 0.1574(13) 0.5976(10) 0.8197(10) 0.018(4) Uani 1 1 d .
O21 O 0.3716(12) 0.7242(10) 0.8715(10) 0.013(3) Uani 1 1 d U
O22 O 0.4886(13) 0.7679(11) 0.7552(11) 0.022(4) Uani 1 1 d U
O23 O 0.3673(13) 0.5080(11) 0.5970(10) 0.021(4) Uani 1 1 d .
O24 O 0.5608(13) 0.6129(12) 0.6474(12) 0.026(4) Uani 1 1 d .
O25 O 0.4393(12) 0.5786(11) 0.7808(10) 0.017(4) Uani 1 1 d U
O26 O 0.2260(13) 0.4571(11) 0.7336(11) 0.022(4) Uani 1 1 d .
O27 O 0.5379(13) 0.6551(11) 0.9616(10) 0.022(4) Uani 1 1 d .
O28 O 0.3043(13) 0.5250(11) 0.8945(11) 0.022(4) Uani 1 1 d U
O29 O 0.6515(12) 0.6946(10) 0.8491(10) 0.017(4) Uani 1 1 d U
O30 O 0.5319(14) 0.4034(13) 0.5913(12) 0.032(5) Uani 1 1 d U
O31 O 0.6002(12) 0.5016(11) 0.7667(10) 0.017(4) Uani 1 1 d U
O32 O 0.4003(13) 0.3909(11) 0.7105(10) 0.019(4) Uani 1 1 d .
O33 O 0.4812(12) 0.4573(11) 0.8813(10) 0.015(4) Uani 1 1 d U
O34 O 0.0090(14) 0.4564(12) 0.6846(12) 0.031(5) Uani 1 1 d .
O35 O 0.4800(14) 1.0526(12) 0.7286(11) 0.029(4) Uani 1 1 d U
O36 O 0.6975(14) 0.5479(12) 0.9398(11) 0.030(5) Uani 1 1 d .
O37 O 0.2859(13) 0.3158(12) 0.8283(12) 0.023(4) Uani 1 1 d .
O38 O 0.3702(13) 0.6922(11) 1.0237(10) 0.017(4) Uani 1 1 d .
O39 O 0.2212(12) 0.7679(10) 0.9453(10) 0.014(4) Uani 1 1 d U
O40 O 0.1564(12) 0.5824(11) 0.9910(10) 0.018(4) Uani 1 1 d .
Si1 Si 0.3983(5) 0.6822(4) 0.7774(4) 0.0077(13) Uani 1 1 d U
W1 W 0.19676(9) 0.77653(7) 0.66827(7) 0.0187(3) Uani 1 1 d .
W2 W 0.47390(9) 0.93209(7) 0.74148(7) 0.0197(3) Uani 1 1 d .
W3 W 0.31021(8) 0.87363(7) 0.90214(7) 0.0170(3) Uani 1 1 d .
W4 W 0.28309(9) 0.59215(7) 0.55451(6) 0.0200(3) Uani 1 1 d .
W5 W 0.13202(8) 0.53753(7) 0.69855(7) 0.0180(3) Uani 1 1 d .
W6 W 0.24572(8) 0.63414(7) 0.93291(6) 0.0152(2) Uani 1 1 d .
W7 W 0.49607(8) 0.77573(7) 1.00373(6) 0.0164(3) Uani 1 1 d .
W8 W 0.66006(8) 0.83241(7) 0.84286(7) 0.0190(3) Uani 1 1 d .
W9 W 0.55988(9) 0.74731(7) 0.62840(7) 0.0212(3) Uani 1 1 d .
W10 W 0.59164(8) 0.57285(7) 0.88054(7) 0.0177(3) Uani 1 1 d .
W11 W 0.49230(9) 0.48628(7) 0.66470(7) 0.0183(3) Uani 1 1 d .
W12 W 0.34305(8) 0.43199(7) 0.80925(7) 0.0157(2) Uani 1 1 d .
Zn1 Zn -0.1239(2) 0.1606(2) 0.6732(2) 0.0254(7) Uani 1 1 d .
Zn2 Zn 0.1532(2) 0.17365(19) 0.78530(19) 0.0200(7) Uani 1 1 d .
Zn3 Zn 0.0000 0.5000 1.0000 0.0568(17) Uani 1 2 d S
N1 N 0.0152(18) 0.2070(15) 0.6219(14) 0.029(3) Uani 1 1 d U
N2 N 0.1180(18) 0.2019(15) 0.6538(14) 0.026(3) Uani 1 1 d U
N3 N 0.1223(18) 0.2694(16) 0.5388(15) 0.033(4) Uani 1 1 d U
H3 H 0.1427 0.2940 0.4966 0.039 Uiso 1 1 calc R
N7 N -0.0429(18) 0.2602(15) 0.7903(14) 0.029(3) Uani 1 1 d U
N8 N 0.0638(18) 0.2685(15) 0.8306(15) 0.029(3) Uani 1 1 d U
N9 N 0.004(2) 0.3818(17) 0.9089(16) 0.041(4) Uani 1 1 d U
N10 N -0.2196(18) 0.0630(15) 0.5593(14) 0.029(3) Uani 1 1 d U
N11 N -0.1903(19) 0.0205(16) 0.4811(15) 0.034(3) Uani 1 1 d U
N12 N -0.3532(19) -0.0429(16) 0.4652(15) 0.034(4) Uani 1 1 d U
H12 H -0.4168 -0.0788 0.4422 0.041 Uiso 1 1 calc R
C1 C 0.021(2) 0.2480(19) 0.5552(19) 0.035(6) Uani 1 1 d U
H1 H -0.0374 0.2616 0.5216 0.042 Uiso 1 1 calc R
C2 C 0.182(3) 0.243(2) 0.6041(19) 0.038(6) Uani 1 1 d U
H2 H 0.2555 0.2518 0.6137 0.045 Uiso 1 1 calc R
C3 C -0.076(2) 0.3266(19) 0.8431(18) 0.033(5) Uani 1 1 d U
H3A H -0.1462 0.3341 0.8358 0.039 Uiso 1 1 calc R
C4 C 0.089(3) 0.345(2) 0.897(2) 0.042(5) Uani 1 1 d U
H4 H 0.1568 0.3708 0.9314 0.051 Uiso 1 1 calc R
C7 C -0.325(2) 0.0189(19) 0.5436(18) 0.030(5) Uani 1 1 d U
H7 H -0.3701 0.0298 0.5814 0.036 Uiso 1 1 calc R
C8 C -0.270(2) -0.0412(18) 0.4279(18) 0.027(4) Uani 1 1 d U
H8 H -0.2696 -0.0779 0.3734 0.033 Uiso 1 1 calc R
N13 N 0.144(2) 0.4555(17) 1.1765(18) 0.079(5) Uani 1 1 d DU
H13 H 0.1791 0.5180 1.1936 0.095 Uiso 1 1 calc R
N15 N 0.084(2) 0.2966(17) 1.1792(19) 0.076(5) Uani 1 1 d DU
C10 C 0.154(3) 0.384(2) 1.2197(19) 0.076(5) Uani 1 1 d DU
H10 H 0.2033 0.3922 1.2713 0.091 Uiso 1 1 calc R
C9 C 0.033(3) 0.3208(19) 1.110(2) 0.072(4) Uani 1 1 d DU
H9 H -0.0242 0.2765 1.0702 0.086 Uiso 1 1 calc R
N16 N 0.075(2) 0.4185(18) 1.1041(16) 0.067(4) Uani 1 1 d DU
O2W O -0.5345(18) -0.1926(14) 0.3944(14) 0.056(7) Uani 1 1 d .
O3W O 0.1296(18) 0.3316(15) 0.3834(15) 0.061(7) Uani 1 1 d .
O4W O -0.364(2) 0.2965(18) 0.7877(16) 0.083(9) Uani 1 1 d .
O5W O 0.003(2) 0.100(2) 0.9802(18) 0.092(10) Uani 1 1 d .
N4 N -0.0712(18) 0.0318(15) 0.7092(14) 0.029(3) Uani 1 1 d U
C5 C -0.123(2) -0.061(2) 0.7073(19) 0.036(6) Uani 1 1 d U
H5 H -0.1938 -0.0876 0.6794 0.043 Uiso 1 1 calc R
N6 N -0.0659(18) -0.1105(16) 0.7476(15) 0.034(4) Uani 1 1 d U
H6 H -0.0860 -0.1713 0.7552 0.041 Uiso 1 1 calc R
N5 N 0.0273(18) 0.0409(15) 0.7549(14) 0.028(3) Uani 1 1 d U
C6 C 0.034(2) -0.046(2) 0.7763(18) 0.034(6) Uani 1 1 d U
H6A H 0.0950 -0.0611 0.8051 0.041 Uiso 1 1 calc R
O1W O -0.2008(19) 0.1147(16) 0.8947(14) 0.064(7) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
W1 O3 W3 150.9(9) . .
W1 O4 W2 151.9(9) . .
W3 O5 W2 154.7(8) . .
W2 O6 W9 122.1(9) . .
W2 O7 W8 122.2(7) . .
Zn1 O6W H6WC 103.8 . .
Zn1 O6W H6WD 118.5 . .
H6WC O6W H6WD 108.1 . .
W1 O8 W5 122.2(8) . .
W3 O9 W7 122.4(8) . .
Zn2 O8W H8WC 112.8 . .
Zn2 O8W H8WD 105.7 . .
H8WC O8W H8WD 108.1 . .
W4 O10 W1 121.8(8) . .
Zn2 O9W H9WC 79.6 . .
W4 O13 W9 151.9(9) . .
W9 O14 W8 122.8(9) . .
W5 O15 W4 121.9(8) . .
Si1 O16 W4 125.1(8) . .
Si1 O16 W1 122.8(8) . .
W4 O16 W1 92.5(5) . .
Si1 O16 W5 123.7(8) . .
W4 O16 W5 91.8(5) . .
W1 O16 W5 91.5(6) . .
W8 O17 W7 152.9(8) . .
W6 O20 W5 150.8(10) . .
Si1 O21 W6 124.3(8) . .
Si1 O21 W7 125.0(8) . .
W6 O21 W7 92.2(5) . .
Si1 O21 W3 122.9(8) . .
W6 O21 W3 92.5(5) . .
W7 O21 W3 90.4(5) . .
Si1 O22 W8 123.1(9) . .
Si1 O22 W2 125.8(9) . .
W8 O22 W2 91.2(5) . .
Si1 O22 W9 124.6(8) . .
W8 O22 W9 91.2(6) . .
W2 O22 W9 90.8(6) . .
W4 O23 W11 152.6(9) . .
W11 O24 W9 151.7(10) . .
Si1 O25 W12 125.4(9) . .
Si1 O25 W11 124.1(9) . .
W12 O25 W11 91.8(5) . .
Si1 O25 W10 122.9(8) . .
W12 O25 W10 90.9(5) . .
W11 O25 W10 91.9(5) . .
W5 O26 W12 153.5(9) . .
W10 O27 W7 152.8(9) . .
W6 O28 W12 154.6(10) . .
W10 O29 W8 153.0(9) . .
W11 O31 W10 122.3(8) . .
W12 O32 W11 122.0(7) . .
W12 O33 W10 120.9(8) . .
W12 O37 Zn2 147.5(10) . .
W7 O38 W6 121.9(8) . .
W6 O39 W3 120.7(8) . .
W6 O40 Zn3 152.0(9) . .
O22 Si1 O25 110.6(9) . .
O22 Si1 O21 109.9(8) . .
O25 Si1 O21 109.0(8) . .
O22 Si1 O16 108.4(8) . .
O25 Si1 O16 108.3(8) . .
O21 Si1 O16 110.6(9) . .
O1 W1 O4 103.6(8) . .
O1 W1 O3 101.7(8) . .
O4 W1 O3 86.8(7) . .
O1 W1 O8 98.1(8) . .
O4 W1 O8 158.3(7) . .
O3 W1 O8 88.1(7) . .
O1 W1 O10 101.4(8) . .
O4 W1 O10 89.0(7) . .
O3 W1 O10 156.8(7) . .
O8 W1 O10 87.5(7) . .
O1 W1 O16 169.3(7) . .
O4 W1 O16 85.2(6) . .
O3 W1 O16 84.7(6) . .
O8 W1 O16 73.4(6) . .
O10 W1 O16 72.2(6) . .
O35 W2 O7 101.0(8) . .
O35 W2 O6 100.8(8) . .
O7 W2 O6 88.9(7) . .
O35 W2 O4 102.2(8) . .
O7 W2 O4 156.7(6) . .
O6 W2 O4 88.6(7) . .
O35 W2 O5 102.0(7) . .
O7 W2 O5 90.1(6) . .
O6 W2 O5 156.9(6) . .
O4 W2 O5 83.2(6) . .
O35 W2 O22 172.3(8) . .
O7 W2 O22 73.8(6) . .
O6 W2 O22 73.7(6) . .
O4 W2 O22 83.3(6) . .
O5 W2 O22 83.9(6) . .
O2 W3 O5 102.3(7) . .
O2 W3 O9 102.2(7) . .
O5 W3 O9 91.9(7) . .
O2 W3 O3 100.8(7) . .
O5 W3 O3 85.2(7) . .
O9 W3 O3 156.9(7) . .
O2 W3 O39 99.7(7) . .
O5 W3 O39 157.7(6) . .
O9 W3 O39 86.9(7) . .
O3 W3 O39 87.1(6) . .
O2 W3 O21 171.1(6) . .
O5 W3 O21 85.9(6) . .
O9 W3 O21 73.7(6) . .
O3 W3 O21 83.2(6) . .
O39 W3 O21 72.4(6) . .
O12 W4 O23 103.8(8) . .
O12 W4 O13 102.7(7) . .
O23 W4 O13 85.4(6) . .
O12 W4 O10 98.7(8) . .
O23 W4 O10 157.5(7) . .
O13 W4 O10 89.0(7) . .
O12 W4 O15 98.9(7) . .
O23 W4 O15 90.4(7) . .
O13 W4 O15 158.3(7) . .
O10 W4 O15 86.9(7) . .
O12 W4 O16 169.1(7) . .
O23 W4 O16 84.4(6) . .
O13 W4 O16 85.0(6) . .
O10 W4 O16 73.4(6) . .
O15 W4 O16 73.4(6) . .
O34 W5 O26 102.3(7) . .
O34 W5 O15 101.7(8) . .
O26 W5 O15 90.2(7) . .
O34 W5 O20 100.8(8) . .
O26 W5 O20 85.2(7) . .
O15 W5 O20 157.5(7) . .
O34 W5 O8 101.4(8) . .
O26 W5 O8 156.1(6) . .
O15 W5 O8 87.7(7) . .
O20 W5 O8 87.7(6) . .
O34 W5 O16 172.0(7) . .
O26 W5 O16 83.8(6) . .
O15 W5 O16 72.8(6) . .
O20 W5 O16 84.8(6) . .
O8 W5 O16 72.9(6) . .
O40 W6 O28 102.7(7) . .
O40 W6 O20 100.0(7) . .
O28 W6 O20 85.2(7) . .
O40 W6 O39 99.4(7) . .
O28 W6 O39 157.8(7) . .
O20 W6 O39 89.7(6) . .
O40 W6 O38 100.8(7) . .
O28 W6 O38 90.4(7) . .
O20 W6 O38 159.2(7) . .
O39 W6 O38 86.6(6) . .
O40 W6 O21 171.6(6) . .
O28 W6 O21 83.6(6) . .
O20 W6 O21 86.0(6) . .
O39 W6 O21 74.5(6) . .
O38 W6 O21 73.4(6) . .
O18 W7 O27 102.4(7) . .
O18 W7 O38 100.5(7) . .
O27 W7 O38 88.3(7) . .
O18 W7 O17 102.7(7) . .
O27 W7 O17 84.4(7) . .
O38 W7 O17 156.7(6) . .
O18 W7 O9 101.6(7) . .
O27 W7 O9 156.0(7) . .
O38 W7 O9 87.7(7) . .
O17 W7 O9 90.0(7) . .
O18 W7 O21 171.4(7) . .
O27 W7 O21 82.8(6) . .
O38 W7 O21 72.6(6) . .
O17 W7 O21 84.5(6) . .
O9 W7 O21 73.5(6) . .
O19 W8 O17 102.7(7) . .
O19 W8 O29 103.5(7) . .
O17 W8 O29 84.9(7) . .
O19 W8 O14 99.2(7) . .
O17 W8 O14 158.1(7) . .
O29 W8 O14 89.1(6) . .
O19 W8 O7 100.1(7) . .
O17 W8 O7 89.9(7) . .
O29 W8 O7 156.4(6) . .
O14 W8 O7 87.2(7) . .
O19 W8 O22 169.4(7) . .
O17 W8 O22 85.4(6) . .
O29 W8 O22 83.8(6) . .
O14 W8 O22 73.0(6) . .
O7 W8 O22 72.8(6) . .
O11 W9 O14 99.5(8) . .
O11 W9 O13 103.9(8) . .
O14 W9 O13 156.5(7) . .
O11 W9 O6 98.6(7) . .
O14 W9 O6 88.4(7) . .
O13 W9 O6 88.9(7) . .
O11 W9 O24 103.3(8) . .
O14 W9 O24 88.8(7) . .
O13 W9 O24 85.0(7) . .
O6 W9 O24 158.0(7) . .
O11 W9 O22 168.8(7) . .
O14 W9 O22 72.9(6) . .
O13 W9 O22 83.9(6) . .
O6 W9 O22 73.3(6) . .
O24 W9 O22 85.1(7) . .
O36 W10 O29 102.7(8) . .
O36 W10 O27 104.7(8) . .
O29 W10 O27 85.9(7) . .
O36 W10 O33 101.0(8) . .
O29 W10 O33 156.3(7) . .
O27 W10 O33 90.1(7) . .
O36 W10 O31 98.7(8) . .
O29 W10 O31 87.5(6) . .
O27 W10 O31 156.6(7) . .
O33 W10 O31 87.0(6) . .
O36 W10 O25 169.5(7) . .
O29 W10 O25 83.0(6) . .
O27 W10 O25 84.4(6) . .
O33 W10 O25 73.3(6) . .
O31 W10 O25 72.5(6) . .
O30 W11 O24 102.3(8) . .
O30 W11 O23 102.5(8) . .
O24 W11 O23 85.2(7) . .
O30 W11 O32 99.5(7) . .
O24 W11 O32 158.1(7) . .
O23 W11 O32 88.0(6) . .
O30 W11 O31 100.8(8) . .
O24 W11 O31 90.2(7) . .
O23 W11 O31 156.7(7) . .
O32 W11 O31 87.9(6) . .
O30 W11 O25 169.9(7) . .
O24 W11 O25 86.1(7) . .
O23 W11 O25 83.7(6) . .
O32 W11 O25 72.5(6) . .
O31 W11 O25 73.2(6) . .
O37 W12 O32 100.7(7) . .
O37 W12 O33 100.0(7) . .
O32 W12 O33 89.5(7) . .
O37 W12 O28 102.8(7) . .
O32 W12 O28 156.3(6) . .
O33 W12 O28 89.8(7) . .
O37 W12 O26 101.2(7) . .
O32 W12 O26 89.1(7) . .
O33 W12 O26 158.7(6) . .
O28 W12 O26 83.1(7) . .
O37 W12 O25 172.2(7) . .
O32 W12 O25 73.6(6) . .
O33 W12 O25 74.9(6) . .
O28 W12 O25 83.3(6) . .
O26 W12 O25 84.3(6) . .
N7 Zn1 N10 174.2(9) . .
N7 Zn1 O6W 88.0(8) . .
N10 Zn1 O6W 86.7(8) . .
N7 Zn1 N1 87.5(9) . .
N10 Zn1 N1 97.6(8) . .
O6W Zn1 N1 172.9(8) . .
N7 Zn1 N4 94.1(8) . .
N10 Zn1 N4 88.5(8) . .
O6W Zn1 N4 93.7(8) . .
N1 Zn1 N4 92.1(8) . .
N7 Zn1 O7W 86.8(9) . .
N10 Zn1 O7W 90.6(9) . .
O6W Zn1 O7W 85.9(8) . .
N1 Zn1 O7W 88.3(9) . .
N4 Zn1 O7W 179.1(9) . .
N8 Zn2 O9W 170.1(8) . .
N8 Zn2 N5 94.9(9) . .
O9W Zn2 N5 94.3(8) . .
N8 Zn2 O8W 86.4(8) . .
O9W Zn2 O8W 89.7(7) . .
N5 Zn2 O8W 91.1(8) . .
N8 Zn2 N2 92.4(8) . .
O9W Zn2 N2 90.9(8) . .
N5 Zn2 N2 92.6(8) . .
O8W Zn2 N2 176.2(7) . .
N8 Zn2 O37 83.1(7) . .
O9W Zn2 O37 87.5(7) . .
N5 Zn2 O37 175.6(8) . .
O8W Zn2 O37 84.9(7) . .
N2 Zn2 O37 91.4(7) . .
N8 Zn2 H9WC 147.6 . .
O9W Zn2 H9WC 23.5 . .
N5 Zn2 H9WC 108.7 . .
O8W Zn2 H9WC 71.6 . .
N2 Zn2 H9WC 108.0 . .
O37 Zn2 H9WC 71.7 . .
N9 Zn3 N9 180 . 2_567
N9 Zn3 O40 91.7(8) . .
N9 Zn3 O40 88.3(8) 2_567 .
N9 Zn3 O40 88.3(8) . 2_567
N9 Zn3 O40 91.7(8) 2_567 2_567
O40 Zn3 O40 180 . 2_567
N9 Zn3 N16 87.6(10) . .
N9 Zn3 N16 92.4(10) 2_567 .
O40 Zn3 N16 91.8(8) . .
O40 Zn3 N16 88.2(8) 2_567 .
N9 Zn3 N16 92.4(10) . 2_567
N9 Zn3 N16 87.6(10) 2_567 2_567
O40 Zn3 N16 88.2(8) . 2_567
O40 Zn3 N16 91.8(8) 2_567 2_567
N16 Zn3 N16 180 . 2_567
C1 N1 N2 105(2) . .
C1 N1 Zn1 127(2) . .
N2 N1 Zn1 127.6(16) . .
C2 N2 N1 108(2) . .
C2 N2 Zn2 131.8(19) . .
N1 N2 Zn2 117.2(16) . .
C2 N3 C1 104(2) . .
C2 N3 H3 128.1 . .
C1 N3 H3 128.1 . .
C3 N7 N8 105(2) . .
C3 N7 Zn1 130(2) . .
N8 N7 Zn1 125.0(17) . .
C4 N8 N7 107(2) . .
C4 N8 Zn2 130(2) . .
N7 N8 Zn2 122.9(16) . .
C4 N9 C3 105(3) . .
C4 N9 Zn3 127(2) . .
C3 N9 Zn3 127(2) . .
C7 N10 N11 102(2) . .
C7 N10 Zn1 128.2(19) . .
N11 N10 Zn1 129.8(16) . .
C8 N11 N10 112(2) . .
C8 N12 C7 110(2) . .
C8 N12 H12 124.8 . .
C7 N12 H12 124.8 . .
N1 C1 N3 113(3) . .
N1 C1 H1 123.4 . .
N3 C1 H1 123.4 . .
N3 C2 N2 109(3) . .
N3 C2 H2 125.3 . .
N2 C2 H2 125.3 . .
N7 C3 N9 111(3) . .
N7 C3 H3A 124.4 . .
N9 C3 H3A 124.4 . .
N8 C4 N9 111(3) . .
N8 C4 H4 124.3 . .
N9 C4 H4 124.3 . .
N12 C7 N10 109(3) . .
N12 C7 H7 125.4 . .
N10 C7 H7 125.4 . .
N11 C8 N12 107(2) . .
N11 C8 H8 126.6 . .
N12 C8 H8 126.6 . .
N16 N13 C10 110.2(18) . .
N16 N13 H13 124.9 . .
C10 N13 H13 124.9 . .
C9 N15 C10 103.0(17) . .
N13 C10 N15 110.5(18) . .
N13 C10 H10 124.8 . .
N15 C10 H10 124.8 . .
N15 C9 N16 112.4(18) . .
N15 C9 H9 123.8 . .
N16 C9 H9 123.8 . .
N13 N16 C9 103.4(17) . .
N13 N16 Zn3 130.6(18) . .
C9 N16 Zn3 124.4(18) . .
C5 N4 N5 105(2) . .
C5 N4 Zn1 132(2) . .
N5 N4 Zn1 122.1(15) . .
N6 C5 N4 113(3) . .
N6 C5 H5 123.4 . .
N4 C5 H5 123.4 . .
C5 N6 C6 105(2) . .
C5 N6 H6 127.3 . .
C6 N6 H6 127.3 . .
C6 N5 N4 109(2) . .
C6 N5 Zn2 125(2) . .
N4 N5 Zn2 125.3(16) . .
N5 C6 N6 107(3) . .
N5 C6 H6A 126.7 . .
N6 C6 H6A 126.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 W1 1.697(17) .
O2 W3 1.717(15) .
O3 W1 1.895(16) .
O3 W3 1.912(16) .
O4 W1 1.886(15) .
O4 W2 1.926(15) .
O5 W3 1.848(15) .
O5 W2 1.936(16) .
O6 W2 1.913(16) .
O6 W9 1.923(17) .
O7 W2 1.885(15) .
O7 W8 1.947(16) .
O6W Zn1 2.137(19) .
O6W H6WC 0.8500 .
O6W H6WD 0.8500 .
O8 W1 1.919(14) .
O8 W5 1.923(15) .
O7W Zn1 2.182(19) .
O9 W3 1.885(15) .
O9 W7 1.925(15) .
O8W Zn2 2.139(18) .
O8W H8WC 0.8500 .
O8W H8WD 0.8499 .
O10 W4 1.904(16) .
O10 W1 1.942(16) .
O9W Zn2 2.080(18) .
O9W H9WC 0.8500 .
O11 W9 1.671(17) .
O12 W4 1.696(16) .
O13 W4 1.888(15) .
O13 W9 1.919(15) .
O14 W9 1.908(15) .
O14 W8 1.926(16) .
O15 W5 1.907(16) .
O15 W4 1.929(16) .
O16 Si1 1.644(17) .
O16 W4 2.313(15) .
O16 W1 2.338(15) .
O16 W5 2.356(15) .
O17 W8 1.879(16) .
O17 W7 1.918(16) .
O18 W7 1.725(16) .
O19 W8 1.703(17) .
O20 W6 1.902(15) .
O20 W5 1.914(15) .
O21 Si1 1.635(16) .
O21 W6 2.307(15) .
O21 W7 2.343(15) .
O21 W3 2.362(14) .
O22 Si1 1.621(16) .
O22 W8 2.346(16) .
O22 W2 2.351(16) .
O22 W9 2.363(17) .
O23 W4 1.887(17) .
O23 W11 1.913(17) .
O24 W11 1.878(15) .
O24 W9 1.927(16) .
O25 Si1 1.629(16) .
O25 W12 2.309(15) .
O25 W11 2.348(15) .
O25 W10 2.361(16) .
O26 W5 1.896(17) .
O26 W12 1.916(17) .
O27 W10 1.891(16) .
O27 W7 1.903(16) .
O28 W6 1.880(16) .
O28 W12 1.910(17) .
O29 W10 1.885(14) .
O29 W8 1.898(14) .
O30 W11 1.711(18) .
O31 W11 1.921(16) .
O31 W10 1.944(16) .
O32 W12 1.905(16) .
O32 W11 1.918(15) .
O33 W12 1.906(16) .
O33 W10 1.922(14) .
O34 W5 1.717(17) .
O35 W2 1.693(15) .
O36 W10 1.675(18) .
O37 W12 1.720(15) .
O37 Zn2 2.253(16) .
O38 W7 1.913(15) .
O38 W6 1.920(15) .
O39 W6 1.915(14) .
O39 W3 1.965(14) .
O40 W6 1.725(14) .
O40 Zn3 2.169(14) .
Zn1 N7 2.09(2) .
Zn1 N10 2.10(2) .
Zn1 N1 2.14(2) .
Zn1 N4 2.16(2) .
Zn2 N8 2.04(2) .
Zn2 N5 2.12(2) .
Zn2 N2 2.19(2) .
Zn2 H9WC 2.1001 .
Zn3 N9 2.00(2) .
Zn3 N9 2.00(2) 2_567
Zn3 O40 2.169(14) 2_567
Zn3 N16 2.35(2) .
Zn3 N16 2.35(2) 2_567
N1 C1 1.29(3) .
N1 N2 1.38(3) .
N2 C2 1.35(3) .
N3 C2 1.34(3) .
N3 C1 1.38(3) .
N3 H3 0.8600 .
N7 C3 1.33(3) .
N7 N8 1.41(3) .
N8 C4 1.30(3) .
N9 C4 1.34(3) .
N9 C3 1.35(3) .
N10 C7 1.35(3) .
N10 N11 1.43(3) .
N11 C8 1.28(3) .
N12 C8 1.32(3) .
N12 C7 1.33(3) .
N12 H12 0.8600 .
C1 H1 0.9300 .
C2 H2 0.9300 .
C3 H3A 0.9300 .
C4 H4 0.9300 .
C7 H7 0.9300 .
C8 H8 0.9300 .
N13 N16 1.299(17) .
N13 C10 1.314(18) .
N13 H13 0.8600 .
N15 C9 1.316(18) .
N15 C10 1.340(18) .
C10 H10 0.9300 .
C9 N16 1.371(18) .
C9 H9 0.9300 .
N4 C5 1.31(3) .
N4 N5 1.34(3) .
C5 N6 1.28(3) .
C5 H5 0.9300 .
N6 C6 1.38(3) .
N6 H6 0.8600 .
N5 C6 1.31(3) .
C6 H6A 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
W8 O22 Si1 O25 -60.2(12) . .
W2 O22 Si1 O25 179.8(9) . .
W9 O22 Si1 O25 58.6(12) . .
W8 O22 Si1 O21 60.2(12) . .
W2 O22 Si1 O21 -59.8(12) . .
W9 O22 Si1 O21 178.9(9) . .
W8 O22 Si1 O16 -178.8(9) . .
W2 O22 Si1 O16 61.2(12) . .
W9 O22 Si1 O16 -60.0(12) . .
W12 O25 Si1 O22 -179.8(9) . .
W11 O25 Si1 O22 -57.9(12) . .
W10 O25 Si1 O22 61.3(12) . .
W12 O25 Si1 O21 59.3(12) . .
W11 O25 Si1 O21 -178.8(8) . .
W10 O25 Si1 O21 -59.7(11) . .
W12 O25 Si1 O16 -61.1(12) . .
W11 O25 Si1 O16 60.8(11) . .
W10 O25 Si1 O16 179.9(8) . .
W6 O21 Si1 O22 178.4(9) . .
W7 O21 Si1 O22 -59.4(11) . .
W3 O21 Si1 O22 58.2(12) . .
W6 O21 Si1 O25 -60.2(12) . .
W7 O21 Si1 O25 62.0(11) . .
W3 O21 Si1 O25 179.5(8) . .
W6 O21 Si1 O16 58.8(11) . .
W7 O21 Si1 O16 -179.0(8) . .
W3 O21 Si1 O16 -61.5(11) . .
W4 O16 Si1 O22 60.0(11) . .
W1 O16 Si1 O22 -61.1(11) . .
W5 O16 Si1 O22 -179.0(9) . .
W4 O16 Si1 O25 -60.0(11) . .
W1 O16 Si1 O25 178.9(8) . .
W5 O16 Si1 O25 61.0(11) . .
W4 O16 Si1 O21 -179.4(8) . .
W1 O16 Si1 O21 59.5(11) . .
W5 O16 Si1 O21 -58.4(11) . .
W2 O4 W1 O1 127(2) . .
W2 O4 W1 O3 26(2) . .
W2 O4 W1 O8 -51(3) . .
W2 O4 W1 O10 -131(2) . .
W2 O4 W1 O16 -59(2) . .
W3 O3 W1 O1 -124.7(19) . .
W3 O3 W1 O4 -21.5(19) . .
W3 O3 W1 O8 137.4(19) . .
W3 O3 W1 O10 58(3) . .
W3 O3 W1 O16 63.9(19) . .
W5 O8 W1 O1 172.6(10) . .
W5 O8 W1 O4 -9(2) . .
W5 O8 W1 O3 -85.9(10) . .
W5 O8 W1 O10 71.4(10) . .
W5 O8 W1 O16 -0.8(8) . .
W4 O10 W1 O1 -170.7(10) . .
W4 O10 W1 O4 85.6(10) . .
W4 O10 W1 O3 6(2) . .
W4 O10 W1 O8 -73.0(10) . .
W4 O10 W1 O16 0.4(8) . .
Si1 O16 W1 O1 -170(4) . .
W4 O16 W1 O1 55(4) . .
W5 O16 W1 O1 -37(4) . .
Si1 O16 W1 O4 44.8(10) . .
W4 O16 W1 O4 -90.7(6) . .
W5 O16 W1 O4 177.4(6) . .
Si1 O16 W1 O3 -42.4(10) . .
W4 O16 W1 O3 -177.9(6) . .
W5 O16 W1 O3 90.2(6) . .
Si1 O16 W1 O8 -132.0(11) . .
W4 O16 W1 O8 92.5(6) . .
W5 O16 W1 O8 0.6(5) . .
Si1 O16 W1 O10 135.2(11) . .
W4 O16 W1 O10 -0.3(6) . .
W5 O16 W1 O10 -92.2(6) . .
W8 O7 W2 O35 -173.0(10) . .
W8 O7 W2 O6 -72.2(9) . .
W8 O7 W2 O4 12(2) . .
W8 O7 W2 O5 84.7(9) . .
W8 O7 W2 O22 1.1(8) . .
W9 O6 W2 O35 172.0(10) . .
W9 O6 W2 O7 71.0(10) . .
W9 O6 W2 O4 -85.8(10) . .
W9 O6 W2 O5 -17(2) . .
W9 O6 W2 O22 -2.4(9) . .
W1 O4 W2 O35 -128(2) . .
W1 O4 W2 O7 47(3) . .
W1 O4 W2 O6 131(2) . .
W1 O4 W2 O5 -27.0(19) . .
W1 O4 W2 O22 58(2) . .
W3 O5 W2 O35 132(2) . .
W3 O5 W2 O7 -126(2) . .
W3 O5 W2 O6 -39(3) . .
W3 O5 W2 O4 31(2) . .
W3 O5 W2 O22 -53(2) . .
Si1 O22 W2 O35 -179(100) . .
W8 O22 W2 O35 47(6) . .
W9 O22 W2 O35 -44(6) . .
Si1 O22 W2 O7 132.7(12) . .
W8 O22 W2 O7 -0.8(6) . .
W9 O22 W2 O7 -92.1(6) . .
Si1 O22 W2 O6 -133.6(12) . .
W8 O22 W2 O6 92.9(7) . .
W9 O22 W2 O6 1.6(6) . .
Si1 O22 W2 O4 -43.1(11) . .
W8 O22 W2 O4 -176.6(7) . .
W9 O22 W2 O4 92.1(6) . .
Si1 O22 W2 O5 40.8(11) . .
W8 O22 W2 O5 -92.7(6) . .
W9 O22 W2 O5 176.0(6) . .
W2 O5 W3 O2 -130(2) . .
W2 O5 W3 O9 127(2) . .
W2 O5 W3 O3 -30(2) . .
W2 O5 W3 O39 40(3) . .
W2 O5 W3 O21 53(2) . .
W7 O9 W3 O2 172.1(9) . .
W7 O9 W3 O5 -84.8(10) . .
W7 O9 W3 O3 -3(2) . .
W7 O9 W3 O39 72.9(10) . .
W7 O9 W3 O21 0.4(8) . .
W1 O3 W3 O2 123.5(19) . .
W1 O3 W3 O5 21.8(19) . .
W1 O3 W3 O9 -62(3) . .
W1 O3 W3 O39 -137.2(19) . .
W1 O3 W3 O21 -64.6(19) . .
W6 O39 W3 O2 -175.7(9) . .
W6 O39 W3 O5 14(2) . .
W6 O39 W3 O9 -73.8(9) . .
W6 O39 W3 O3 83.8(9) . .
W6 O39 W3 O21 0.1(8) . .
Si1 O21 W3 O2 162(4) . .
W6 O21 W3 O2 28(4) . .
W7 O21 W3 O2 -64(4) . .
Si1 O21 W3 O5 -40.5(10) . .
W6 O21 W3 O5 -174.9(6) . .
W7 O21 W3 O5 92.9(6) . .
Si1 O21 W3 O9 -133.6(11) . .
W6 O21 W3 O9 91.9(7) . .
W7 O21 W3 O9 -0.3(6) . .
Si1 O21 W3 O3 45.2(10) . .
W6 O21 W3 O3 -89.2(6) . .
W7 O21 W3 O3 178.6(6) . .
Si1 O21 W3 O39 134.4(11) . .
W6 O21 W3 O39 0.0(5) . .
W7 O21 W3 O39 -92.2(6) . .
W11 O23 W4 O12 129(2) . .
W11 O23 W4 O13 27(2) . .
W11 O23 W4 O10 -49(3) . .
W11 O23 W4 O15 -132(2) . .
W11 O23 W4 O16 -59(2) . .
W9 O13 W4 O12 -130.3(19) . .
W9 O13 W4 O23 -27.2(19) . .
W9 O13 W4 O10 131(2) . .
W9 O13 W4 O15 52(3) . .
W9 O13 W4 O16 57.5(19) . .
W1 O10 W4 O12 171.8(9) . .
W1 O10 W4 O23 -10(2) . .
W1 O10 W4 O13 -85.4(10) . .
W1 O10 W4 O15 73.3(10) . .
W1 O10 W4 O16 -0.4(8) . .
W5 O15 W4 O12 -172.2(10) . .
W5 O15 W4 O23 83.8(10) . .
W5 O15 W4 O13 5(2) . .
W5 O15 W4 O10 -73.9(10) . .
W5 O15 W4 O16 -0.3(8) . .
Si1 O16 W4 O12 -179(3) . .
W1 O16 W4 O12 -45(3) . .
W5 O16 W4 O12 47(3) . .
Si1 O16 W4 O23 42.6(10) . .
W1 O16 W4 O23 176.5(6) . .
W5 O16 W4 O23 -91.9(6) . .
Si1 O16 W4 O13 -43.2(10) . .
W1 O16 W4 O13 90.7(6) . .
W5 O16 W4 O13 -177.7(6) . .
Si1 O16 W4 O10 -133.6(11) . .
W1 O16 W4 O10 0.3(6) . .
W5 O16 W4 O10 91.9(6) . .
Si1 O16 W4 O15 134.7(11) . .
W1 O16 W4 O15 -91.4(7) . .
W5 O16 W4 O15 0.2(6) . .
W12 O26 W5 O34 -128(2) . .
W12 O26 W5 O15 130(2) . .
W12 O26 W5 O20 -28.4(19) . .
W12 O26 W5 O8 45(3) . .
W12 O26 W5 O16 56.9(19) . .
W4 O15 W5 O34 174.3(10) . .
W4 O15 W5 O26 -83.1(10) . .
W4 O15 W5 O20 -5(2) . .
W4 O15 W5 O8 73.1(10) . .
W4 O15 W5 O16 0.3(8) . .
W6 O20 W5 O34 128.5(17) . .
W6 O20 W5 O26 26.9(16) . .
W6 O20 W5 O15 -52(3) . .
W6 O20 W5 O8 -130.3(17) . .
W6 O20 W5 O16 -57.3(16) . .
W1 O8 W5 O34 -173.4(10) . .
W1 O8 W5 O26 13(2) . .
W1 O8 W5 O15 -71.9(10) . .
W1 O8 W5 O20 86.1(10) . .
W1 O8 W5 O16 0.8(8) . .
Si1 O16 W5 O34 177(4) . .
W4 O16 W5 O34 -48(5) . .
W1 O16 W5 O34 45(5) . .
Si1 O16 W5 O26 -43.5(10) . .
W4 O16 W5 O26 92.0(6) . .
W1 O16 W5 O26 -175.4(6) . .
Si1 O16 W5 O15 -135.7(11) . .
W4 O16 W5 O15 -0.2(6) . .
W1 O16 W5 O15 92.4(7) . .
Si1 O16 W5 O20 42.2(10) . .
W4 O16 W5 O20 177.7(6) . .
W1 O16 W5 O20 -89.8(6) . .
Si1 O16 W5 O8 131.4(11) . .
W4 O16 W5 O8 -93.1(6) . .
W1 O16 W5 O8 -0.6(5) . .
Zn3 O40 W6 O28 -87(2) . .
Zn3 O40 W6 O20 0(2) . .
Zn3 O40 W6 O39 91(2) . .
Zn3 O40 W6 O38 179.6(19) . .
Zn3 O40 W6 O21 134(4) . .
W12 O28 W6 O40 127(2) . .
W12 O28 W6 O20 28(2) . .
W12 O28 W6 O39 -50(3) . .
W12 O28 W6 O38 -132(2) . .
W12 O28 W6 O21 -59(2) . .
W5 O20 W6 O40 -128.6(16) . .
W5 O20 W6 O28 -26.5(16) . .
W5 O20 W6 O39 131.9(16) . .
W5 O20 W6 O38 52(3) . .
W5 O20 W6 O21 57.4(16) . .
W3 O39 W6 O40 174.0(9) . .
W3 O39 W6 O28 -9(2) . .
W3 O39 W6 O20 -85.9(9) . .
W3 O39 W6 O38 73.6(9) . .
W3 O39 W6 O21 -0.1(8) . .
W7 O38 W6 O40 -172.9(9) . .
W7 O38 W6 O28 84.0(10) . .
W7 O38 W6 O20 6(2) . .
W7 O38 W6 O39 -74.0(10) . .
W7 O38 W6 O21 0.8(8) . .
Si1 O21 W6 O40 -178(4) . .
W7 O21 W6 O40 46(5) . .
W3 O21 W6 O40 -44(5) . .
Si1 O21 W6 O28 43.1(10) . .
W7 O21 W6 O28 -93.0(6) . .
W3 O21 W6 O28 176.6(7) . .
Si1 O21 W6 O20 -42.5(10) . .
W7 O21 W6 O20 -178.6(6) . .
W3 O21 W6 O20 90.9(6) . .
Si1 O21 W6 O39 -133.4(11) . .
W7 O21 W6 O39 90.5(6) . .
W3 O21 W6 O39 0.0(5) . .
Si1 O21 W6 O38 135.5(11) . .
W7 O21 W6 O38 -0.6(6) . .
W3 O21 W6 O38 -91.1(6) . .
W10 O27 W7 O18 -125(2) . .
W10 O27 W7 O38 135(2) . .
W10 O27 W7 O17 -23(2) . .
W10 O27 W7 O9 54(3) . .
W10 O27 W7 O21 62(2) . .
W6 O38 W7 O18 173.9(10) . .
W6 O38 W7 O27 -83.8(10) . .
W6 O38 W7 O17 -12(2) . .
W6 O38 W7 O9 72.6(10) . .
W6 O38 W7 O21 -0.8(8) . .
W8 O17 W7 O18 130(2) . .
W8 O17 W7 O27 29(2) . .
W8 O17 W7 O38 -44(3) . .
W8 O17 W7 O9 -128(2) . .
W8 O17 W7 O21 -54(2) . .
W3 O9 W7 O18 -173.2(10) . .
W3 O9 W7 O27 8(2) . .
W3 O9 W7 O38 -72.9(10) . .
W3 O9 W7 O17 83.9(10) . .
W3 O9 W7 O21 -0.4(8) . .
Si1 O21 W7 O18 -172(4) . .
W6 O21 W7 O18 -37(5) . .
W3 O21 W7 O18 56(4) . .
Si1 O21 W7 O27 -44.5(10) . .
W6 O21 W7 O27 91.1(6) . .
W3 O21 W7 O27 -176.4(6) . .
Si1 O21 W7 O38 -135.0(11) . .
W6 O21 W7 O38 0.6(6) . .
W3 O21 W7 O38 93.1(6) . .
Si1 O21 W7 O17 40.5(10) . .
W6 O21 W7 O17 176.2(6) . .
W3 O21 W7 O17 -91.3(6) . .
Si1 O21 W7 O9 132.1(11) . .
W6 O21 W7 O9 -92.2(7) . .
W3 O21 W7 O9 0.2(6) . .
W7 O17 W8 O19 -131(2) . .
W7 O17 W8 O29 -29(2) . .
W7 O17 W8 O14 46(3) . .
W7 O17 W8 O7 128(2) . .
W7 O17 W8 O22 56(2) . .
W10 O29 W8 O19 124(2) . .
W10 O29 W8 O17 22(2) . .
W10 O29 W8 O14 -137(2) . .
W10 O29 W8 O7 -56(3) . .
W10 O29 W8 O22 -64(2) . .
W9 O14 W8 O19 -171.6(9) . .
W9 O14 W8 O17 11(2) . .
W9 O14 W8 O29 84.8(10) . .
W9 O14 W8 O7 -71.9(9) . .
W9 O14 W8 O22 1.0(8) . .
W2 O7 W8 O19 170.8(9) . .
W2 O7 W8 O17 -86.3(9) . .
W2 O7 W8 O29 -9(2) . .
W2 O7 W8 O14 72.0(9) . .
W2 O7 W8 O22 -1.1(8) . .
Si1 O22 W8 O19 176(3) . .
W2 O22 W8 O19 -48(4) . .
W9 O22 W8 O19 43(4) . .
Si1 O22 W8 O17 -43.2(10) . .
W2 O22 W8 O17 92.1(6) . .
W9 O22 W8 O17 -177.0(6) . .
Si1 O22 W8 O29 42.1(10) . .
W2 O22 W8 O29 177.5(7) . .
W9 O22 W8 O29 -91.6(6) . .
Si1 O22 W8 O14 133.1(11) . .
W2 O22 W8 O14 -91.5(6) . .
W9 O22 W8 O14 -0.7(6) . .
Si1 O22 W8 O7 -134.6(11) . .
W2 O22 W8 O7 0.8(5) . .
W9 O22 W8 O7 91.6(6) . .
W8 O14 W9 O11 170.5(9) . .
W8 O14 W9 O13 -12(2) . .
W8 O14 W9 O6 72.0(10) . .
W8 O14 W9 O24 -86.2(10) . .
W8 O14 W9 O22 -1.0(8) . .
W4 O13 W9 O11 130.6(19) . .
W4 O13 W9 O14 -47(3) . .
W4 O13 W9 O6 -131(2) . .
W4 O13 W9 O24 28(2) . .
W4 O13 W9 O22 -57.5(19) . .
W2 O6 W9 O11 -169.7(11) . .
W2 O6 W9 O14 -70.3(10) . .
W2 O6 W9 O13 86.4(10) . .
W2 O6 W9 O24 12(3) . .
W2 O6 W9 O22 2.4(9) . .
W11 O24 W9 O11 -133(2) . .
W11 O24 W9 O14 128(2) . .
W11 O24 W9 O13 -30(2) . .
W11 O24 W9 O6 45(3) . .
W11 O24 W9 O22 55(2) . .
Si1 O22 W9 O11 179(3) . .
W8 O22 W9 O11 -48(4) . .
W2 O22 W9 O11 43(4) . .
Si1 O22 W9 O14 -132.0(12) . .
W8 O22 W9 O14 0.7(6) . .
W2 O22 W9 O14 91.9(6) . .
Si1 O22 W9 O13 43.7(11) . .
W8 O22 W9 O13 176.4(6) . .
W2 O22 W9 O13 -92.4(6) . .
Si1 O22 W9 O6 134.5(12) . .
W8 O22 W9 O6 -92.8(7) . .
W2 O22 W9 O6 -1.6(6) . .
Si1 O22 W9 O24 -41.8(11) . .
W8 O22 W9 O24 90.9(6) . .
W2 O22 W9 O24 -177.9(7) . .
W8 O29 W10 O36 -125(2) . .
W8 O29 W10 O27 -21(2) . .
W8 O29 W10 O33 60(3) . .
W8 O29 W10 O31 137(2) . .
W8 O29 W10 O25 64(2) . .
W7 O27 W10 O36 124(2) . .
W7 O27 W10 O29 22(2) . .
W7 O27 W10 O33 -135(2) . .
W7 O27 W10 O31 -52(3) . .
W7 O27 W10 O25 -62(2) . .
W12 O33 W10 O36 -170.8(9) . .
W12 O33 W10 O29 4(2) . .
W12 O33 W10 O27 84.2(9) . .
W12 O33 W10 O31 -72.6(9) . .
W12 O33 W10 O25 0.1(7) . .
W11 O31 W10 O36 173.8(9) . .
W11 O31 W10 O29 -83.7(9) . .
W11 O31 W10 O27 -10(2) . .
W11 O31 W10 O33 73.2(9) . .
W11 O31 W10 O25 -0.3(7) . .
Si1 O25 W10 O36 -167(4) . .
W12 O25 W10 O36 58(4) . .
W11 O25 W10 O36 -33(4) . .
Si1 O25 W10 O29 -43.8(10) . .
W12 O25 W10 O29 -178.3(6) . .
W11 O25 W10 O29 89.8(6) . .
Si1 O25 W10 O27 42.7(10) . .
W12 O25 W10 O27 -91.8(6) . .
W11 O25 W10 O27 176.4(6) . .
Si1 O25 W10 O33 134.5(11) . .
W12 O25 W10 O33 -0.1(5) . .
W11 O25 W10 O33 -91.9(6) . .
Si1 O25 W10 O31 -133.4(11) . .
W12 O25 W10 O31 92.0(6) . .
W11 O25 W10 O31 0.2(5) . .
W9 O24 W11 O30 131(2) . .
W9 O24 W11 O23 29(2) . .
W9 O24 W11 O32 -43(3) . .
W9 O24 W11 O31 -128(2) . .
W9 O24 W11 O25 -54(2) . .
W4 O23 W11 O30 -129(2) . .
W4 O23 W11 O24 -28(2) . .
W4 O23 W11 O32 132(2) . .
W4 O23 W11 O31 52(3) . .
W4 O23 W11 O25 59(2) . .
W12 O32 W11 O30 170.9(10) . .
W12 O32 W11 O24 -15(2) . .
W12 O32 W11 O23 -86.8(10) . .
W12 O32 W11 O31 70.3(10) . .
W12 O32 W11 O25 -2.8(8) . .
W10 O31 W11 O30 -171.2(9) . .
W10 O31 W11 O24 86.2(9) . .
W10 O31 W11 O23 8(2) . .
W10 O31 W11 O32 -72.0(9) . .
W10 O31 W11 O25 0.3(7) . .
Si1 O25 W11 O30 -173(4) . .
W12 O25 W11 O30 -36(4) . .
W10 O25 W11 O30 55(4) . .
Si1 O25 W11 O24 41.2(11) . .
W12 O25 W11 O24 177.4(7) . .
W10 O25 W11 O24 -91.6(7) . .
Si1 O25 W11 O23 -44.3(10) . .
W12 O25 W11 O23 91.9(6) . .
W10 O25 W11 O23 -177.1(6) . .
Si1 O25 W11 O32 -134.3(12) . .
W12 O25 W11 O32 1.9(6) . .
W10 O25 W11 O32 92.9(6) . .
Si1 O25 W11 O31 132.6(11) . .
W12 O25 W11 O31 -91.2(6) . .
W10 O25 W11 O31 -0.2(5) . .
Zn2 O37 W12 O32 -72.0(17) . .
Zn2 O37 W12 O33 -163.4(16) . .
Zn2 O37 W12 O28 104.6(17) . .
Zn2 O37 W12 O26 19.2(18) . .
Zn2 O37 W12 O25 -115(5) . .
W11 O32 W12 O37 -171.6(10) . .
W11 O32 W12 O33 -71.6(10) . .
W11 O32 W12 O28 17(2) . .
W11 O32 W12 O26 87.1(10) . .
W11 O32 W12 O25 2.8(8) . .
W10 O33 W12 O37 173.9(9) . .
W10 O33 W12 O32 73.1(9) . .
W10 O33 W12 O28 -83.2(9) . .
W10 O33 W12 O26 -13(2) . .
W10 O33 W12 O25 -0.1(8) . .
W6 O28 W12 O37 -127(2) . .
W6 O28 W12 O32 45(3) . .
W6 O28 W12 O33 133(2) . .
W6 O28 W12 O26 -27(2) . .
W6 O28 W12 O25 58(2) . .
W5 O26 W12 O37 129(2) . .
W5 O26 W12 O32 -130(2) . .
W5 O26 W12 O33 -44(3) . .
W5 O26 W12 O28 27.5(19) . .
W5 O26 W12 O25 -56.4(19) . .
Si1 O25 W12 O37 178(5) . .
W11 O25 W12 O37 43(5) . .
W10 O25 W12 O37 -49(5) . .
Si1 O25 W12 O32 133.4(12) . .
W11 O25 W12 O32 -2.0(6) . .
W10 O25 W12 O32 -93.9(7) . .
Si1 O25 W12 O33 -132.6(11) . .
W11 O25 W12 O33 92.0(6) . .
W10 O25 W12 O33 0.1(5) . .
Si1 O25 W12 O28 -41.0(11) . .
W11 O25 W12 O28 -176.4(7) . .
W10 O25 W12 O28 91.6(6) . .
Si1 O25 W12 O26 42.7(11) . .
W11 O25 W12 O26 -92.7(6) . .
W10 O25 W12 O26 175.3(6) . .
W12 O37 Zn2 N8 -73.2(18) . .
W12 O37 Zn2 O9W 109.8(18) . .
W12 O37 Zn2 N5 -136(9) . .
W12 O37 Zn2 O8W -160.2(18) . .
W12 O37 Zn2 N2 19.0(18) . .
W6 O40 Zn3 N9 55(2) . .
W6 O40 Zn3 N9 -125(2) . 2_567
W6 O40 Zn3 O40 -59(30) . 2_567
W6 O40 Zn3 N16 143(2) . .
W6 O40 Zn3 N16 -37(2) . 2_567
N7 Zn1 N1 C1 -121(2) . .
N10 Zn1 N1 C1 56(2) . .
O6W Zn1 N1 C1 -71(7) . .
N4 Zn1 N1 C1 145(2) . .
O7W Zn1 N1 C1 -34(2) . .
N7 Zn1 N1 N2 57(2) . .
N10 Zn1 N1 N2 -125.7(19) . .
O6W Zn1 N1 N2 107(6) . .
N4 Zn1 N1 N2 -37(2) . .
O7W Zn1 N1 N2 144(2) . .
C1 N1 N2 C2 1(3) . .
Zn1 N1 N2 C2 -177.4(18) . .
C1 N1 N2 Zn2 164.8(17) . .
Zn1 N1 N2 Zn2 -14(2) . .
N8 Zn2 N2 C2 118(2) . .
O9W Zn2 N2 C2 -53(2) . .
N5 Zn2 N2 C2 -147(2) . .
O8W Zn2 N2 C2 47(13) . .
O37 Zn2 N2 C2 35(2) . .
N8 Zn2 N2 N1 -40.8(17) . .
O9W Zn2 N2 N1 148.6(16) . .
N5 Zn2 N2 N1 54.2(17) . .
O8W Zn2 N2 N1 -112(12) . .
O37 Zn2 N2 N1 -123.9(16) . .
N10 Zn1 N7 C3 -17(9) . .
O6W Zn1 N7 C3 -39(2) . .
N1 Zn1 N7 C3 135(2) . .
N4 Zn1 N7 C3 -133(2) . .
O7W Zn1 N7 C3 47(2) . .
N10 Zn1 N7 N8 162(7) . .
O6W Zn1 N7 N8 139.9(19) . .
N1 Zn1 N7 N8 -45.6(19) . .
N4 Zn1 N7 N8 46.2(19) . .
O7W Zn1 N7 N8 -134.1(19) . .
C3 N7 N8 C4 -7(3) . .
Zn1 N7 N8 C4 173.7(19) . .
C3 N7 N8 Zn2 173.5(17) . .
Zn1 N7 N8 Zn2 -6(3) . .
O9W Zn2 N8 C4 -18(6) . .
N5 Zn2 N8 C4 140(3) . .
O8W Zn2 N8 C4 49(3) . .
N2 Zn2 N8 C4 -127(3) . .
O37 Zn2 N8 C4 -36(3) . .
O9W Zn2 N8 N7 161(4) . .
N5 Zn2 N8 N7 -40.5(19) . .
O8W Zn2 N8 N7 -131.3(19) . .
N2 Zn2 N8 N7 52.3(19) . .
O37 Zn2 N8 N7 143.4(19) . .
N9 Zn3 N9 C4 117(100) 2_567 .
O40 Zn3 N9 C4 37(3) . .
O40 Zn3 N9 C4 -143(3) 2_567 .
N16 Zn3 N9 C4 -55(3) . .
N16 Zn3 N9 C4 125(3) 2_567 .
N9 Zn3 N9 C3 -58(100) 2_567 .
O40 Zn3 N9 C3 -138(2) . .
O40 Zn3 N9 C3 42(2) 2_567 .
N16 Zn3 N9 C3 130(3) . .
N16 Zn3 N9 C3 -50(3) 2_567 .
N7 Zn1 N10 C7 -18(9) . .
O6W Zn1 N10 C7 5(2) . .
N1 Zn1 N10 C7 -170(2) . .
N4 Zn1 N10 C7 98(2) . .
O7W Zn1 N10 C7 -81(2) . .
N7 Zn1 N10 N11 167(7) . .
O6W Zn1 N10 N11 -171(2) . .
N1 Zn1 N10 N11 15(2) . .
N4 Zn1 N10 N11 -77(2) . .
O7W Zn1 N10 N11 103(2) . .
C7 N10 N11 C8 0(3) . .
Zn1 N10 N11 C8 175.6(18) . .
N2 N1 C1 N3 1(3) . .
Zn1 N1 C1 N3 179.8(16) . .
C2 N3 C1 N1 -3(3) . .
C1 N3 C2 N2 4(3) . .
N1 N2 C2 N3 -3(3) . .
Zn2 N2 C2 N3 -163.5(17) . .
N8 N7 C3 N9 6(3) . .
Zn1 N7 C3 N9 -175.3(18) . .
C4 N9 C3 N7 -2(3) . .
Zn3 N9 C3 N7 174.0(18) . .
N7 N8 C4 N9 6(3) . .
Zn2 N8 C4 N9 -174.4(18) . .
C3 N9 C4 N8 -3(3) . .
Zn3 N9 C4 N8 -178.8(18) . .
C8 N12 C7 N10 0(3) . .
N11 N10 C7 N12 0(3) . .
Zn1 N10 C7 N12 -175.9(17) . .
N10 N11 C8 N12 0(3) . .
C7 N12 C8 N11 0(3) . .
N16 N13 C10 N15 -5(5) . .
C9 N15 C10 N13 1(5) . .
C10 N15 C9 N16 4(5) . .
C10 N13 N16 C9 6(4) . .
C10 N13 N16 Zn3 173(3) . .
N15 C9 N16 N13 -6(5) . .
N15 C9 N16 Zn3 -174(3) . .
N9 Zn3 N16 N13 143(3) . .
N9 Zn3 N16 N13 -37(3) 2_567 .
O40 Zn3 N16 N13 51(3) . .
O40 Zn3 N16 N13 -129(3) 2_567 .
N16 Zn3 N16 N13 -39(100) 2_567 .
N9 Zn3 N16 C9 -53(3) . .
N9 Zn3 N16 C9 127(3) 2_567 .
O40 Zn3 N16 C9 -145(3) . .
O40 Zn3 N16 C9 35(3) 2_567 .
N16 Zn3 N16 C9 125(100) 2_567 .
N7 Zn1 N4 C5 130(3) . .
N10 Zn1 N4 C5 -45(3) . .
O6W Zn1 N4 C5 42(3) . .
N1 Zn1 N4 C5 -142(3) . .
O7W Zn1 N4 C5 -29(60) . .
N7 Zn1 N4 N5 -38(2) . .
N10 Zn1 N4 N5 148(2) . .
O6W Zn1 N4 N5 -125.7(19) . .
N1 Zn1 N4 N5 50(2) . .
O7W Zn1 N4 N5 164(58) . .
N5 N4 C5 N6 0(3) . .
Zn1 N4 C5 N6 -168.9(19) . .
N4 C5 N6 C6 -2(3) . .
C5 N4 N5 C6 3(3) . .
Zn1 N4 N5 C6 172.9(18) . .
C5 N4 N5 Zn2 -178.9(19) . .
Zn1 N4 N5 Zn2 -9(3) . .
N8 Zn2 N5 C6 -132(2) . .
O9W Zn2 N5 C6 44(2) . .
O8W Zn2 N5 C6 -46(2) . .
N2 Zn2 N5 C6 135(2) . .
O37 Zn2 N5 C6 -70(10) . .
N8 Zn2 N5 N4 49(2) . .
O9W Zn2 N5 N4 -134(2) . .
O8W Zn2 N5 N4 136(2) . .
N2 Zn2 N5 N4 -43(2) . .
O37 Zn2 N5 N4 111(9) . .
N4 N5 C6 N6 -4(3) . .
Zn2 N5 C6 N6 177.5(17) . .
C5 N6 C6 N5 4(3) . .
